I mixed a cone 6 porcelain body and a cone 6 clear glaze 50:50 and added 10% Mason 6666 black stain. The material was plastic enough to slurry, dewater and wedge like a clay, so I dried a slab and broke it up into small pieces. I then melted them at cone 6 in a zircopax crucible (I make these by mixing alumina or zircopax with veegum and throwing them on the wheel). Because this black material does not completely melt it is easy to break the crucible away from it. As you can see no zircon sticks to the black. I then break this up with a special flat metal crusher we made, size them on sieves and add them to glazes for artificial speckle. As it turned out, this mix produced specks that fused too much, so a lower percentage of glaze is needed. I can thus fine tune the recipe and particle size to theoretically duplicate the appearance of reduction speckle.
In reduction firing, where insufficient oxygen is present to oxidize the iron, natural iron pyrite particles in the clay convert to their metallic form and melt. The nature of the decorative speckled effect depends on the size of the particles, the distribution of sizes, their abundance, the color of the clay and the degree to which they melt. The characteristics of the glaze on the ware (e.g. degree of matteness, color, thickness of application, the way it interacts with the iron) also have a big effect on the appearance.
|Recipes||G2934 - Matte Glaze Base for Cone 6
A base MgO matte glaze recipe fires to a hard utilitarian surface and has very good working properties. Blend in the glossy if it is too matte.
A sought-after visual effect that occurs in reduction fired stoneware. Particles of iron pyrite that occur naturally in the clay melt and blossom up through the glaze
Dolomite matte glazes have the potential to be very silky and pleasant to the touch, while at the same time being hard, durable and non-crazed (if they are formulated correctly).